- Open Access
The use of ECT and 6PBP tests to evaluate fracture behavior of adhesively bonded steel/epoxy joints under Mode-III and Mixed Mode III/II
© Asgari Mehrabadi; licensee Springer. 2014
Received: 29 November 2013
Accepted: 27 January 2014
Published: 7 May 2014
Evaluation of fracture energy of adhesive joints under mode-III and mixed-mode III/II is a key issue when failure analyses have to be performed. It is thus useful to determine fracture toughness under mode-III and characterization of crack front behavior of bonded joints under mixed-mode III/II loading conditions, which were the overall goal of this paper. For this purpose, edge crack torsion (ECT) and six-point bending plate (6PBP) tests were employed using steel/epoxy adhesive joint. The experimental tests were performed under displacement control and three types of configurations were tested to achieve different mixed-mode ratios. Test results showed considerable linearity before the maximum load point both under pure mode III and mixed-mode III/II; also, failure examination indicated that dominate failure under tearing mode was adhesive/adherend interface, which will be discussed in detail. The experimental tests were numerically simulated and virtual crack closure technique (VCCT) was employed to reproduce behavior of crack front propagation. Both experimental compliance method and finite element analysis proved applicable for the fracture mechanism of adhesive assemblies under mode-III and mixed-mode III/II.
Structural bonding is now a well-known assembly technique used in many industrial sectors which includes aerospace, automobiles, electrical, electronics, packaging, etc. Adhesive bonding offers considerable advantages compared with traditional forms of joining, such as bolting, riveting, and welding like giving high stiffness, strength and fatigue life, easily being automated and not requiring secondary operations for surface finishing to attain smooth exterior surfaces which result in time and cost efficiency. In the transportation industry and more specifically in the aerospace and automotive industries, this assembly technique is now used to:
Improve energy management capability and enable using advanced high strength steel,
Enable down-gauged steel and multi-material construction,
Reduce the number of spot-welds, and
Improve acoustics by increasing stiffness of the structure body, durability by overcoming fatigue problems and longtime durability by an anticorrosion barrier.
A particular issue with the integrity of adhesive joints is the presence of cracks and flaws in the as-manufactured adhesive bond-line. The presence of these defects, at least in some scales, seems inevitable and propagation of such cracks/flaws has the potential of affecting the service life of the adhesively bonded joints and even causing catastrophic failure of bonded structures in service. Hence, a better understanding of crack propagation behavior under realistic types of combined (in-out of plane shear stress components) service loading is an important aspect of evaluating the potential performance of adhesively bonded joints.
In principle, crack propagation can be described using a fracture mechanics approach. Fracture characterization of bonded joints under pure mode-I has been extensively studied by several authors. Double cantilever beam (DCB) and tapered DCB (TDCB) tests are the most widely used methods for measuring mode-I fracture toughness [1–4]. Three-point bending of adhesively bonded end notched flexure (ENF) has shown to be the preferred test technique for obtaining mode-II critical strain energy release rate [5–9]. Mode-II crack propagation has received some attention with the development of four-point bend end-notch flexure (4ENF) and end-loaded split (ELS) [5, 10], which induce stable crack propagation.
As is known, crack growth could occur in any ratio of mode-I and II components of the strain energy release rate. Therefore, in addition to the pure mode tests, mixed-mode crack propagation tests have to be also carried out. The mixed-mode bending (MMB) test is now the most widely used method for investigating mixed-mode I/II fracture behavior [15–17]. This test is a combination of DCB test (pure mode I fracture) and ENF test (pure mode-II fracture), which allows for studying any combination of modes I and II. Arcan test is another useful method that has been previously employed to evaluate mixed-mode I/II fracture behavior of bonded assemblies .
Numerous works have been published on characterizing the performance of adhesive joints under mode-I, mode-II and mixed-mode I/II loading; however, they have not provided a basis for conservative and safe design under more complex loadings. Hence, the need for more complicated fracture characterization becomes unavoidable.
To the best knowledge of the present author, little mode-III and mixed-mode III/II experiments on fracture behavior of adhesive bonded joints have been reported in the literature [19–23]. Therefore, the objective of this study was to investigate mode-III and mixed-mode III/II fracture properties of adhesively bonded steel/epoxy joints. For this purpose, modification of the ECT specimen was used as proposed by Li  and 6PBP specimen  was employed to evaluate mode III and mixed-mode III/II in order. The strain energy release rate distribution along the crack advance front was analyzed using a three-dimensional finite element model. The stress intensity factors for ECT and 6PBP specimens were also investigated using finite element analysis.
Mechanical properties of adhesive
Tensile strength at 25°C (MPa)
Lap Shear strength (MPa)
Adhesive (epoxy AD-314)
Type I: S = 140 mm, d = 35 mm.
Type II: S = 120 mm, d = 55 mm.
Type III: S = 90 mm, d = 70 mm.
For each joint type, three specimens were examined under ambient laboratory conditions. Axial compression loads were applied using a universal testing machine (GOTECH AL-7000L) with 10 kN load cell capacity. All the specimens were loaded up to failure in the displacement rate of 0.5 mm/min. This slow rate allowed crack propagation to be stable so that fracture process zone (FPZ) in crack tip can be form slowly to avoid unstable crack advance.
In the case of mixed-mode III/II, the basic idea behind the development of the present test was to generate both modes by bending . In these circumstances, 6PBP specimens (Figure 3(b)) were considered a reasonable solution for creating mixed-mode crack growth III/II. According to Figure 3, a special rig transferred bending load on both sides of specimen while the specimen rested on 4 mid-supports; so, it was seen that this configuration promoted crack advances near the edges (along mid-plane of adhesive layer). Furthermore, it was able to generate high mode-III and mode-II when high S and small d values (Figure 2) were adopted. Also, it seemed that 6PBP test was a useful and simple test for characterizing the mixed-mode III/II fracture of bonded assemblies.
ECT and 6PBP tests were conducted to determine the load–displacement behavior and the mode-III and mixed-mode III/II fracture behaviors of adhesive joints.
where B is the specimen width, a the crack length obtained with the applied load P and corresponding displacement δ, and C the specimen compliance. Standard methods for the SERR calculation are based on this equation, the difference between them basically being the way in which the derivative dC/da is obtained.
The method used in this study is the compliance calibration method which employs a multi-specimen compliance calibration procedure. In this paper, the method is called CC method.
where μxy,0 and μxy,1 designate the classical lamination theory (CLT) torsional shear moduli of the uncracked and cracked parts of the specimen, respectively.
Naturally, mode-III condition using ECT is more complex than in modes I and II fracture tests which requires specimens with different crack lengths. In fact, the crack position cannot be monitored during ECT tests and the crack length cannot be varied by repositioning a single specimen. However, this method bears errors inherent to specimen variability and increases substantially test costs. In order to overcome those drawbacks, a new data reduction scheme based on the compliance versus crack length relation is proposed by de Moura et al. . Other problems may affect mode-III and mixed-mode III/II tests, e.g. identifying correctly the initiation failure point. The commonly employed non-linearity and maximum load criteria can give substantially different results.
Therefore, considerable research is still needed to validate the ECT and 6PBP tests for measuring G IIIc of adhesive joints. The present study aimed at evaluating its adequacy for adhesively bonded steel/epoxy joints by combining numerical analyses and experimental tests.
3D finite element models were established for the ECT and 6PBP specimens using the software ANSYS.12 . A typical crack, as schematically illustrated in Figure 1, was introduced in the FEA models between the mid-plane of adhesive layers. The element type SOLID45 was used and, based on a parametric study, a mesh size of 0.4 mm for the crack increment (∆a) was selected for both joint types. In order to avoid the mutual penetration of the adherends in mode III and mixed-mode fracture, the correlated contact (CONTA174) and target (TARGE170) elements were employed for the two crack surfaces. The ECT model comprised 4680 elements and the 6PBP model 5520 elements. The boundary conditions of the testing configuration were simulated so that were the same as those illustrated in Figures 1 and 2. Experimental load values corresponding to arbitrarily selected crack lengths were used as input for calculation of the corresponding nodal displacements and forces. Non-linear-elastic analysis (for existing of contact elements) was performed and the specimen elongations, nodal forces and nodal displacements were calculated. Also, based on parametric study, mesh fine and type of elements (using more higher order elements) do not affected on values of nodal force and displacements on crack tip and in order to model the specimens in this paper, just around the crack tip and along the crack over width of the specimens, the finer mesh has been used for VCC method.
Results and Discussions
Fracture loads of ECT and 6PBP tests
6PBP (a 0 = 30 mm)
a 0 = 10 mm
a 0 = 15 mm
a 0 = 20 mm
a 0 = 25 mm
a 0 = 30 mm
Failure load (N)
Mean value (N)
ECT and 6PBP tests were repeated at least three times for each crack length and loading mode ratios, respectively. Then, average values of critical maximum loads were extracted to be employed in FE analysis (Table 2). Moreover, no plastic deformation was observed in the adherends after unloading and all the tested samples were essentially linear elastic to failure.
This failure was mostly observed in pure mode-III tests where the crack path switched into the interface. Actually, crack kinking was a significant observation in the ECT test so that almost in all the studied specimens, the initial crack in the adhesive layer quickly turned and propagated along the adhesive/adherend interface, which was probably caused by creating mode-III (tearing) helping torsion of the specimen during the test.
Typically, fracture test method requires obtaining three critical strain energy release rate values. The first one is based on the load where the load–displacement curve first deviates from linearity (non-linear), F NL . The second option is based on the maximum load, F max , and the third one corresponds to the point at which the actual crack initiation is visually observed by the testing personnel.
In this section, the loads corresponding to crack initiation in the ECT specimen are used to calculate the critical strain energy release rates through the width of specimen using non-linear elastic finite element models. Computational approaches like FEMs play an important role in detecting mechanical crack front and damage of adhesive assemblies.
Moreover, Figure 9 indicates that mode-III component was approximately constant over the central region of ECT specimens. However, the plateau size presenting the amount of mode-III component remained sensibly at the same level, meaning that distribution of strain energy release rates could not explain the crack length dependence of GIIIc. Similarly, crack front in mode-I showed such a behavior in adhesive joints and composite materials such as SERR had the maximum and minimum values in the middle width of adhesive layer and at edges, respectively; leaving the edges, SERR increased and approached a constant value (plateau region) and decreased while getting closer to the edges [34–36].
In spite of mode-I and mode-III, crack front distribution in mode-II was uniform with the exception of localized peaks at the specimen edge [36, 37] and crack advance was linear and no difference was detected between crack length at the edges and in the center of the specimen. This point demonstrated that, in mode-III as mode-I loading, there was a higher potential for the growth of crack in the center width of adhesive pad, which indicated that a crack can grow in mode-I and mode-III without being noticed.
This issue should be designated in designing an adhesive joint. Also, this behavior can be seen in mode-I and mode-III interlaminar fractures of multidirectional laminates .
Furthermore, numerical results indicated that, in 6PBP test, mode-III and mode-II components can be created by controlling load and support points. Also, comparison of fracture load showed that fracture load decreased with changing mixed-mode ratio (mode-III to mode-II dominate). Nonetheless, the 6PBP test for mixed-mode III/II condition inevitably involved the non-uniform distribution of crack growth and it was also clear that mixed-mode III/II fracture required extensive investigation which should lead to the development of improved test methods.
The results indicated that the proposed fixture (modified ECT and 6PBP tests) could be very useful for creating mode-III and mixed-mode III/II crack growth conditions for adhesive bonded joints so that an optimum configuration could give 96% mode-III contribution to the total energy release rate.
Based on the fracture surface examination, adhesive/adherend interface failure was the dominant failure and combination of adhesive and cohesive failure was achieved in ECT and 6PBP tests, respectively, which indicated that cohesive failure occurred when mode-II components dominated fracture state in 6PBP test.
It was shown that GIII increased with the crack length increase using compliance method whereas mode-I and mode-II critical fracture energy showed a stable resistant curve (R-curve).
The finite element results showed almost stable crack growth under mode-III loading, meaning that the distribution of critical strain energy release rates could not explain crack length dependence of G IIIC .
Also, numerical analysis proved that 6PBP test had non-uniform distribution of G II and G III which resulted in non-uniform crack advance and depended on finite element methods. Also, propagation of crack initiation can be mostly estimated between load and support points.
The author wishes to thank the Institute of Standard (Arak, Iran) and Mr. A. Azizi for kindly provided access to their facilities for experimental tests.
- Steinbrecher G, Buchman A, Sidess A, Sherman D: Characterization of the mode I fracture energy of adhesive joints. Int J Adhes Adhes 2006, 26: 644–650. 10.1016/j.ijadhadh.2005.09.006View ArticleGoogle Scholar
- Ashcroft IA, Hughes DJ, Shaw SJ: Mode I fracture of epoxy bonded composite joints:1. Quasi static loading. Int J Adhes Adhes 2001, 21: 87–99. 10.1016/S0143-7496(00)00038-5View ArticleGoogle Scholar
- Blackman BRK, Kinloch AJ, Paraschi M, Teo WS: Measuring the mode I adhesive fracture energy, GIC, of structural adhesive joints: the results of an international round-robin. Int J Adhes Adhes 2001, 23: 293–305.View ArticleGoogle Scholar
- de Moura MFSF, Campilho RDSG, Gonçalves JPM: Crack equivalent concept applied to the fracture characterization of bonded joints under pure mode I loading. Comp Sci Tech 2008, 68: 2224–2230. 10.1016/j.compscitech.2008.04.003View ArticleGoogle Scholar
- Blackman BRK, Kinloch AJ, Paraschi M: The determination of the mode II adhesive fracture resistance, GIIC, of structural adhesive joints: an effective crack length approach. Eng Frac Mech 2005, 72: 877–897. 10.1016/j.engfracmech.2004.08.007View ArticleGoogle Scholar
- de Moura MFSF, Campilho RDSG, Gonçalves JPM: Pure mode II fracture characterization of composite bonded joints. Int J Solids Struct 2009, 46: 1589–1595. 10.1016/j.ijsolstr.2008.12.001View ArticleGoogle Scholar
- Kim WS, Lee JJ: Fracture characterization of interfacial cracks with frictional contact of the crack surfaces to predict failures in adhesive-bonded joints. Eng Frac Mech 2009, 76: 1785–1799. 10.1016/j.engfracmech.2009.03.014View ArticleGoogle Scholar
- Carlsson LA, Gillespie JW, Pipes RB: On the analysis and design of end notched flexure (ENF) specimen for measuring mode II fracture toughness. J Compos Mater 1986, 20: 594–604. 10.1177/002199838602000606View ArticleGoogle Scholar
- de Moura MFSF, Gonçalves JPM, Chousal JAG, Campilho RDSG: Cohesive and continuum mixed-mode damage models applied to the simulation of the mechanical behaviour of bonded joints. Int J Adhes Adhes 2008, 28: 419–426. 10.1016/j.ijadhadh.2008.04.004View ArticleGoogle Scholar
- Yoshihara H, Mode II: R-curve of wood measured by 4-ENF test. Eng Frac Mech 2004, 71: 2065–2077. 10.1016/j.engfracmech.2003.09.001View ArticleGoogle Scholar
- Dollhofer J, Beckert W, Lauke B, Schneider K: Fracture mechanics characterization of mixed-mode toughness of thermoplast/glass interfaces (brittle/ductile interfacial mixed-mode fracture). J Adh Sci Technol 2001, 15: 1559–1587. 10.1163/156856101753207689View ArticleGoogle Scholar
- Shahin K, Taheri F: Fracture behaviour of adhesively bonded joints in sandwich composite beams. J Adh Sci Technol 2009, 23: 1531–1546. 10.1163/156856109X433054View ArticleGoogle Scholar
- Pao YH, Morman KN, Dickie RA: On the effect of an interfacial layer on the fracture behavior of interface and subinterface cracks in single-lap shear joints. J Adh Sci Technol 1990, 4: 503–520. 10.1163/156856190X00469View ArticleGoogle Scholar
- States DN, DeVries KL: Geometric factors impacting adhesive Lap joint strength and design. J Adh Sci Technol 2012, 26: 89–107.Google Scholar
- Hafiz TA, Wahab MMA, Crocombe AD, Smith PA: Mixed-mode fracture of adhesively bonded metallic joints under quasi-static loading. Eng Frac Mech 2010, 77: 3434–3445. 10.1016/j.engfracmech.2010.09.015View ArticleGoogle Scholar
- Ameli A, Papini M, Schroeder JA, Spelt JK: Fracture R-curve characterization of toughened epoxy adhesives. Eng Frac Mech 2010, 77: 521–534. 10.1016/j.engfracmech.2009.10.009View ArticleGoogle Scholar
- Balzani C, Wagner W, Wilckens D, Degenhardt R, Busing S, Reimerdes HG: Adhesive joints in composite laminates-A combined numerical/experimental estimate of critical energy release rates. Int J Adhes Adhes 2012, 32: 23–38.Google Scholar
- Choupani N: Interfacial mixed-mode fracture characterization of adhesively bonded joints. Int J Adhes Adhes 2008, 28: 267–282. 10.1016/j.ijadhadh.2007.08.002View ArticleGoogle Scholar
- Sharif F, Kortschot MT, Martin RH: Mode III delamination using a split cantilever beam, composite materials. Fatigue Fracture 1995, 5: ASTM STP1230.Google Scholar
- Fernlund G, Lanting H, Spelt JK: Mixed mode II/III fracture of adhesive joints. J Compos Technol Res 1995, 17: 317–330. 10.1520/CTR10452JView ArticleGoogle Scholar
- Lanting H, Spelt JK: Shear fracture of adhesively-bonded rigid elements. Compos Part B 1997, 28: 319–329. 10.1016/S1359-8368(96)00033-9View ArticleGoogle Scholar
- Vintilescu I, Spelt JK: Mixed-mode I-II-III fracture characterization of adhesive joints. J Compos Technol Res 1998, 20: 129–139. 10.1520/CTR10053JView ArticleGoogle Scholar
- Vintilescu I, Spelt JK: Fracture load prediction of adhesive joints under mixed-mode I-II-III conditions. J Compos Technol Res 1998, 20: 187–197. 10.1520/CTR10851JView ArticleGoogle Scholar
- Li J, Lee SM, Lee EW, Brien TKO: Evaluation of the edge crack torsion (ECT) test for mode III interlaminar fracture toughness of laminated composites. J Compos Technol Res 1997, 19: 174–183. 10.1520/CTR10028JView ArticleGoogle Scholar
- de Morais AB, Pereira AB: Mixed mode II + III interlaminar fracture of carbon/epoxy laminates. Compos Sci Technol 2008, 68: 2022–2027. 10.1016/j.compscitech.2008.02.023View ArticleGoogle Scholar
- Mokarrar Industrial group database . Accessed 21 February 2012 http://www.mokarrar.com . Accessed 21 February 2012
- Marat-Mendes R, de Freitas M: Characterization of the edge crack torsion (ECT) test for the measurement of the mode III interlaminar fracture toughness. Eng Frac Mech 2009, 76: 2799–2809. 10.1016/j.engfracmech.2009.06.016View ArticleGoogle Scholar
- Anderson TL: Fracture mechanics: fundamentals and applications. Boca Raton: CRC press; 1995.Google Scholar
- Lee SM: An edge crack torsion method for mode III delamination fracture testing. J Compos Tech Res 1993, 15: 193–201. 10.1520/CTR10369JView ArticleGoogle Scholar
- de Moura MFSF, Fernandez MVC, de Morais AB, Campilho RDSG: Numerical analysis of the edge crack torsion test for mode III interlaminar fracture of composite laminates. Eng Frac Mech 2009, 76: 469–478. 10.1016/j.engfracmech.2008.10.004View ArticleGoogle Scholar
- Ansys: ANSYS Release 12.0 Documentation. Pennsylvania, USA: Ansys Inc; 2009.Google Scholar
- Krueger R: The Virtual Crack-Closure Technique: History, Approach and Applications. In NASA/CR-2002–211628, ICASE Report No. 2002–10. Hampton, Virginia, USA: NASA Langley Research Center; 2002.Google Scholar
- Asgari Mehrabadi F, Khoshravan M: Mode III interlaminar fracture and damage characterization in woven fabric-reinforced glass/epoxy composite laminates. J Compos Mater 2013, 47: 1583–1592. 10.1177/0021998312449770View ArticleGoogle Scholar
- Khoshravan M, Asgari Mehrabadi F: Fracture analysis in adhesive composite material/aluminum joints under mode-I loading; experimental and numerical approaches. Int J Adhes Adhes 2012, 39: 8–14.View ArticleGoogle Scholar
- Pereira AB, de Morais AB, de Moura MFSF, Magalhães AG: Mode I interlaminar fracture of woven glass/epoxy multidirectional laminates. Compos Part A 2005, 36: 1119–1127. 10.1016/j.compositesa.2005.01.006View ArticleGoogle Scholar
- Pereira AB, de Morais AB: Mixed mode I + II interlaminar fracture of carbon/epoxy laminates. Compos Part A 2008, 39: 322–333. 10.1016/j.compositesa.2007.10.013View ArticleGoogle Scholar
- de Moura MFSF, Silva MAL, de Morais AB, Morais JJL: Equivalent crack based mode II fracture characterization of wood. Eng Fract Mech 2006, 73: 978–993. 10.1016/j.engfracmech.2006.01.004View ArticleGoogle Scholar
- Szekrényes A: Improved analysis of the modified split-cantilever beam for mode-III fracture. Int J Mech Sci 2009, 51: 682–693. 10.1016/j.ijmecsci.2009.07.005View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.